- Open Access
HRTEM low dose: the unfold of the morphed graphene, from amorphous carbon to morphed graphenes
© The Author(s) 2016
- Received: 16 March 2016
- Accepted: 5 August 2016
- Published: 22 August 2016
We present experimental evidence under low-dose conditions transmission electron microscopy for the unfolding of the evolving changes in carbon soot during mechanical milling. The milled soot shows evolving changes as a function of the milling severity or time. Those changes are responsible for the transformation from amorphous carbon to graphenes, graphitic carbon, and highly ordered structures such as morphed graphenes, namely Rh6 and Rh6-II. The morphed graphenes are corrugated layers of carbon with cross-linked covalently nature and sp2- or sp3-type allotropes. Electron microscopy and numerical simulations are excellent complementary tools to identify those phases. Furthermore, the TEAM 05 microscope is an outstanding tool to resolve the microstructure and prevent any damage to the sample. Other characterization techniques such as XRD, Raman, and XPS fade to convey a true identification of those phases because the samples are usually blends or mixes of the mentioned phases.
- Fast Fourier Transformation
- Zone Axis
- Milling Time
- Graphitic Carbon
- Carbon Nanostructures
Research in the discovery of carbon nanostructures (CNs) have resulted in two nobel prices: one for the fullerene [1, 2] and the second one for the graphene [3, 4]. These and other CNs are carbon allotropes with nanoscale dimensions (e.g., nanotube, nano onions, etc. [5, 6]). Graphene and the nanotubes are the most interesting when compared to other CNs due to its potential in a wide variety of applications that are derived by its physical properties [7–9]. Thus far, the reported CNs are sp2 bonded, except for diamond that is sp3 [10, 11]. CNs are complex in nature and require sophisticated/dedicated manufacturing infrastructure with rather unfortunately low yields (mg/h) [3, 8, 12–16]. These technological limitations have delayed the true industrialization and commercialization of CNs. Most CNs are relatively good conductors (band gap = 0 eV) except for graphene and diamond that may be considered the best conductors (thermal and electrical) ever discovered [3, 4, 17–19]. Some CNs have shown narrow band gaps in doped (<0.53 eV) [20–23] or in zigzag nanotubes [24, 25]. One of the newly identified phases (Rh6) is a natural semiconductor that makes it unique and worth researching it. We envision that this phase has great potential for electronic and optical applications.
Identification of carbon allotropes is quite complicated due to the large variety of carbon phases and the pronounced effects of even subtle morphology changes as in the twisted layer graphene [26, 27]. The characteristics of the morphed graphenes have been previously predicted numerically  and more recently we have proposed their existence . However, there is still a great discrepancy regarding the morphed graphenes (Rh6 and Rh6-II). Here is where the use of electron microscopy becomes important since there should not be any beam-induced damage to the sample so that the genuine crystalline structure and atomic arrangement can be preserved. Additionally until now, the yield of those phases is rather limited and they are normally blends. This combination makes their detection and identification with Raman or other characterization methods (e.g., XRD, XPS, etc.) rather complicated. In the past, those phases have been misidentified as nanodiamonds . Sophisticated ab initio simulations have been carried out to make sure that our findings are correct . We synthesize those structures in a green, friendly, solid-state process [31–33].
Our raw material is the fullerene soot or leftover byproduct from the Krätschmer method . The raw material is a commercial product called fullerene soot which is a consequent leftover material once fullerene is extracted . In this work, batches of 2 g have been milled using a SPEX 8000 M mixer/mill. The milling times have been varied from 0 to 50 h using hardened steel media. Milling times of 50 h or more can contribute to ~2 wt% Fe contamination. Fe is removed using a super magnet and an acid wash (1 h in 6 M HNO3) in an ultrasonic bath followed by an ethanol wash. The acid procedure is repeated 5 times.
The characterization includes an X-ray diffraction (XRD), Raman, and high-resolution transmission electron microscopy (HRTEM). The HRTEM is carried in the TEAM 05 tool located at NCEM-LBNL California under low-dose conditions. The dose rate is normally reduced by using the monochromator attached to the microscope, in order to shift the beam without introducing any sort of aberrations, to less than 200 e−/Å2s for single images and to around 20 e−/Å2s for images in focal series.
A focal series consists of 40 images taken with an exposure time of 1 s and at different focus settings; between each image, there is a waiting time of approximately 1 s. Thus, the total dose in a focal series reaches approximately 800 e−/Å2. Such a dose is sufficiently low to prevent damage as a result of beam sample interaction in this investigation. The TEAM 0.5 has been used at 80 kV and aligned to reach a C3 (Cs) aberration coefficient of −0.015 mm with a focus spread of approximately 10 Å. A normal alignment of the TEAM 0.5 has been done by keeping aberrations such as C1, A1, A2, B2, A3, S3, A4, D4, B4, C5, and A5 within the confidence limits of measurement and keeping C3 at the specified value. The conditions have been earlier tested in different materials including graphene [34–36] to image the genuine atomic arrangement of the sample by preventing any damage and keeping the required resolution of the investigated material.
The CNs phases that we can produce include graphene, graphitic carbon, Rh6, and Rh6-II. The synthesis evolution from amorphous carbon to the morphed graphenes is summarized as follows: amorphous soot (raw), graphene (2–3 layers), graphitic carbon (4–10+ layers), and morphed graphenes (Rh6 and Rh6-II). We are well familiar with amorphous soot and graphene; however, here we will focus on the morphed graphenes that are the product of cold welding during milling . The patent of our process is currently in process .
The most intriguing observation is the existence of a morphed structure of Rh6-II type. While the morphing from graphene to Rh6 preserves the sp2 bonding, the one to Rh6-II rotates the existing bonds and makes new ones thus changing the bonding character from sp2 to sp3 (Fig. 2). The development of this transformation sponsors the sp3 bonding that has been monitored using XPS. The content of sp3 in the raw soot is approximately 4.2 wt% and it increases to 18.25 wt% sp3 bonding in a sample milled for 20 h of milling. Based on the XPS results, we have an approximate ratio between sp2 and sp3 of 4.5:1. Some of the sp2 belongs to the amorphous carbon and part of the sp3 is attributed to dangling bonds; perhaps ~4.2 wt% sp3 or slightly more is measured in the raw sample. We attribute this increase in the sp3 bonding to the change in nature of the carbon during the morphing from the graphene structures into the non-graphitic or Rh6-II. Yet, there is a critical time (e.g., 20 h) that allows to maximize the presence of sp3 and after that it decays.
On a final note, we need to mention that we have the evidence of the first CNs that has a morphing mechanism from sp2 to sp3. A feasibility to detect them using Raman spectroscopy is of paramount importance. Unfortunately, the amounts that we have obtained thus far do not allow us to obtain clear spectra of either phase (e.g., Rh6 or Rh6-II). Therefore, the Raman spectra for the pure phases cannot be resolved due to overlapping of the Raman bands. We have simulated (ab initio using CASTEP) the Raman active modes for Rh6 and Rh6-II structures and compared to preliminary results. Therefore, we have presented experimental evidence for morphed graphene nanostructures in which the carbon–carbon bonding is predominantly sp2 (Rh6) or sp3 (Rh6-II) type.
Since there are no other observable reflections of graphite in XRD or the FFT-SAEDP (Fig. 1a), we proposed that the soot has limited order in the “c” direction and no order in the “a” directions. Raman spectroscopy supports the XRD results (Fig. 1d) by the intense D band in the soot. The D band is typical of nanosized or amorphous carbon. The G band suggests a graphitic structure and the weak 2D band indicates that the honeycomb structure is only short range. This combination of features is common in carbon structures with limited order.
Samples were milled from 1 to 50 h and their characterization results were carried out to illustrate the structural changes that occurred in the materials. The main goal is to identify the effect of milling during the synthesis of this new allotrope. In our previous work we reported the existance of those structures [30, 41, 42, 44–46] based on diamond-like polytypes known as 2H and 4H in  that are proposed numerically. Here we present the analysis of samples where we show the evidence that these are new carbon nanostructures and should not be confused with neither diamond nor graphitic structures. Instead, we identify them as new nanostructures of carbon that are morphed stacks of graphene and therefore we name them morphed graphene.
Identification of phases using the FFT-SAEDP from the images presented in Fig. 6
In Fig. 2b, the Raman spectra for the milled samples for different times are presented. Within short times (0.5–2 h), the 2D band develops, implying that graphene and/or graphitic carbon are still present. Further milling times fade away the well-developed 2D band. The structure of the samples milled for longer times is hard to identify by Raman due to the lack of clarity on the changes, except for features that are present below the 900 cm−1. Those features are of interest because graphitic structures are not active in those ranges. In our ab initio simulations for the Rh6 and Rh6-II (Fig. 2c, d) structures, it is observed activity in those regions.
Atomic resolution microscopy and HRTEM are mandatory in this work in order to unfold the characteristics of the as-milled phases. In the following we present the results of low-dose transmission electron microscopy made in the TEAM 05 microscope. The TEAM 05 is selected for this work in principle due to its high stability and development to prevent beam damage by reducing the electron beam dose rate with the use of the integrated monochromator.
The DFT calculations were performed on the ab initio plane-wave pseudopotential code CASTEP . The GGA was used to account for exchange and correlation in the Perdew–Burke–Ernzerhof (PBE) form . Both atom positions and the unit cell were relaxed to minimize the atomic forces and the total energy, such that forces were converged to 0.001 eV/A and stress residual to 0.002 GPa. A plane-wave cutoff of 310 eV was used, and Brillouin-Zone integrals were performed using a 4 × 4 × 10 Monkhort-Pack grid . The Raman spectra for all the carbon polymorphs were obtained from CASTEP package using norm-conserving pseudopotentials (energy cutoff 310 eV) and the PBE-GGA exchange correlation functional.
Three different areas/particles have been analyzed in Fig. 6. They are selected on the basis of their crystalline appearance. They are abundant in the as-milled products which is evident in the added image (Fig. 6a). The area observed in Fig. 6b has three domains which are analyzed separately using a Fast Fourier Transformation (FFT) analysis in the Digital Micrograph® software. The FFT-SAEDPs are used to confirm the d-spacing with a higher statistics than direct measurements on specific areas along the particles. In other words, measuring the d-spacing in the FFT-SAEDP is more accurate and recommended. Each of the small roman numbers corresponds to a particle that is identified in Table 1. The particles identified as (i), (ii) belong to phase RH6, while area (iii) to Rh6-II. This identification is conducted based on our results and the d-spacing that is compared to the ab initio simulations for the XRD spectra.
The reflections from the FFT are matched against those d-spacing and miller indices as per the ab initio simulations. The experimental results are compared in Table 1. In Table 1, , the first two (i and ii) of the three selected particles belong to the Rh6 phase and the third one belongs to Rh6-II. The respective miller indices are provided within the table along with their respective d-spacing. It is important to point out that the reported d-spacing was measured directly over the FFT diffraction pattern to improve accuracy and the values were further confirmed measuring directly on the HRTEM images. The results can be compared to those in Fig. 4. Additionally, the identified reflections in (iii) are secondary reflections, it means they are repeated planes diffracting at the respective locations. This information is used here as example to show the uniqueness of each of the particles. In addition, this allows us to demonstrate that the non-graphitic structures (seen as crystalline regions in Fig. 6) are not graphite or graphitic carbon and each one is different in nature. Furthermore, the presence of the crystalline areas is not limited to the spot analyzed in Fig. 6a. Instead, we show in Fig. 5 a large number of locations with the crystalline areas.
Figure 7 shows the experimental images of each involved area together with an inset showing the image simulation for a defocus setting near 0 nm. The corresponding FFTs are also shown, they have been used to determine the corresponding zone axis and for phase identification. The small insets in each experimental image clearly match the image features for the selected defocus setting. This is possible only for the selected phases and the respective crystalline structure and zone axis, allowing phase identification in these particular areas. In this manner, area (i) is identified as a result of observation along a zone axis near  as the RH6 phase. Results for area (ii) are given in Fig. 7b; here the nearest zone axis is along [−1−14]. This is a zone axis rather close to a high symmetry axis in the structure of Rh6 but slightly tilted away. The magnification of the image still allows observing a network of columns in two directions but with rather small spacings between them. The image simulation in this case has been done for the precise [−1−14] orientation and only straight bars are obtained.
Figure 7c shows the results for area (iii). In this case, the zone axis is determined to be  for the phase RH6-II. The image simulation is overlapped on the filtered experimental area (iii) image to improve the quality and ease the comparison. Filtering the IFFT-HRTEM image helped demonstrating the almost perfect match between experimental and simulated results. Filtering only involves removing low frequencies in the FFT.
The existence of the morphed structure Rh6-II is quite novel due to its bonding rotation from sp2 to sp3, which is further confirmed with XPS. The percentage of sp2 decreases from 95 to 81 wt% for the raw and milled products, respectively. At the same time, the presence of sp3 increases from 4.2 wt% sp3 to 18.2 at% sp3 for the raw and milled soot for 20 h. After that the abundance drops to 8.7 wt% sp3 in the sample milled for 50 h. The XPS results detect up to 0.7 at% Fe for samples milled up to 20 h, which is a contamination caused by wearing of the milling media. The contamination after 50 h of milling increased to approximately 3 wt%. What we can learn from the XPS results is that the presence of sp3 bonds increases with milling times, which we attributed it to an increase in Rh6-II.
This is important evidence because we can appreciate a particle that is breaking into two new ones. We believe that highly deformed graphenes are the initial state to develop morphed graphenes. In Fig. 9 are identified three regions as (i), (ii), and (iii) with their respective FFTs. In the three regions, we measured the d-spacing directly over the image and we identify the following values: (i) 0.359, (ii) 0.35, and (iii) 0.337 nm. The d-spacing can also be determined using the FFT (inset) for the reciprocal distances (1), (2), and (3) with the following results: 0.363, 0.354, and 0.332 nm. From both measurements, we can conclude that the values from each approach are close confirming their differences. Using the values reported in Fig. 4, we conclude that the d-spacings are for the planes (110), (101), and (002) for the corresponding Rh6-II, Rh6, and graphitic structures. The d-spacings in 4a and 4b are 0.20 and 0.218 nm, which are the perpendicular distance. Based on this evidence, we conclude that the plastic deformation during milling sponsors the transformation of graphene into Rh6 and then at higher levels of deformation Rh6 may transform into the Rh6-II structure. Nevertheless, the development of a phase such as Rh6 ii does not have to depend on a sequence but rather on the bonding and thus on the very different possibilities that a highly aleatory processing such as mechanical milling can offer.
The same d-spacings and differences were measured with conventional HRTEM images and XRD, con1cluding that in order to achieve the right accuracy to interpret the results, we needed an instrument with higher resolution. Here is where the resolution on the TEAM 05 is key because it is clearly evident that the fine differences among the results presented could not be resolved with conventional instruments.
We have presented the HRTEM evidence under low dose for conventional structures of carbon (graphene and graphitic carbon) as well as the newly identified carbon nanostructures known as morphed graphenes. The use of atomic resolution TEM is of paramount interest because it is the only characterization tool available to distinguish the differences among Rh6 and Rh6-II. The nanostructures have been predicted previously and some features are identified using Raman, XRD, and XPS, but neither of those methods has been capable of proving the existence of the aforementioned phases. Here a complementary set of experimental and numerical tools is used to clearly demonstrate the presence of the two morphed graphene phases and their uniqueness when compare to graphene or other carbon allotropes. Furthermore, electron microscopy investigations in low-dose conditions are key to allow a thorough characterization of the morphed graphenes, while preserving them in damage-free condition (intact).
HAC carried the HRTEM, simulations, discussions, analysis of results and manuscript preparation. AO sample preparation and characterization. IEG sample preparation and characterization. VGH Raman characterization, simulations, discussions and analysis of results. FAR simulations, analysis of results, FCRH ideas, experiments, sample preparation, analysis of results, and manuscript preparation. All authors read and approved the final manuscript.
IEG thanks the CONACYT support under project 169262. VGH work was supported by the State of Texas through the Texas Center for Superconductivity (TcSUH) at the University of Houston. HACB wishes to acknowledge the use of electron microscopes at NCEM of the Molecular Foundry (Lawrence Berkeley National Laboratory), which was supported by the Office of Science, the Office of Basic Energy Sciences, the U.S. Department of Energy under Contract No. DE-AC02-05CH11231. HACB also acknowledges CONACYT (Grant 129207 and 148304) and IPN (COFAA).
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Kroto, H.W., et al.: C60: buckminsterfullerene. Nature 318(6042), 162–163 (1985)View ArticleGoogle Scholar
- Kratschmer, W., et al.: Solid C60: a new form of carbon. Nature 347(6291), 354–358 (1990)View ArticleGoogle Scholar
- Geim, A.K., Novoselov, K.S.: The rise of graphene. Nat. Mater. 6(3), 183–191 (2007)View ArticleGoogle Scholar
- Novoselov, K.S., et al.: Electric field effect in atomically thin carbon films. Science 306(5696), 666–669 (2004)View ArticleGoogle Scholar
- Umadevi, D., Sastry, G.N.: Molecular and ionic interaction with graphene nanoflakes: a computational investigation of CO2, H2O, Li, Mg, Li + , and Mg2 + interaction with polycyclic aromatic hydrocarbons. The Journal of Physical Chemistry C 115(19), 9656–9667 (2011)View ArticleGoogle Scholar
- Shenderova, O., Brenner, D., Ruoff, R.S.: Would diamond nanorods be stronger than fullerene nanotubes? Nano Lett. 3(6), 805–809 (2003)View ArticleGoogle Scholar
- Warner, J.H., et al.: Graphene fundamentals to applications, 1st edn. Elsevier, Amsterdam. p (2013). 450 Google Scholar
- Choi, W., Lee, J.-w.: Graphene: synthesis and applications. Nanomaterials and their applications. CRC Press, Boca Raton. xv, p. 347, 8 p. of plates (2012)Google Scholar
- Guldi, D.M., Martin, N.: Carbon nanotubes and related structures: synthesis, characterization, functionalization, and applications. Wiley, Weinheim (2010). 539 View ArticleGoogle Scholar
- Ferrari, A.C., Robertson, J.: Raman spectroscopy of amorphous, nanostructured, diamond-like carbon, and nanodiamond. Philos Trans A Math Phys Eng Sci 2004(362), 2477–2512 (1824)Google Scholar
- Dresselhaus, M.S., Jorio, A., Saito, R.: Characterizing graphene, graphite, and carbon nanotubes by Raman spectroscopy. Ann Rev Condens Matter Phys 1(1), 89–108 (2010)View ArticleGoogle Scholar
- Eizenberg, M., Blakely, J.M.: Carbon interaction with nickel surfaces—monolayer formation and structural stability. J Chem Phys 71(8), 3467–3477 (1979)View ArticleGoogle Scholar
- Li, X.S., et al.: Large-area synthesis of high-quality and uniform graphene films on copper foils. Science 324(5932), 1312–1314 (2009)View ArticleGoogle Scholar
- Berger, C., et al.: Ultrathin epitaxial graphite: 2D electron gas properties and a route toward graphene-based nanoelectronics. J Phys Chem B 108(52), 19912–19916 (2004)View ArticleGoogle Scholar
- Stankovich, S., et al.: Synthesis of graphene-based nanosheets via chemical reduction of exfoliated graphite oxide. Carbon 45(7), 1558–1565 (2007)View ArticleGoogle Scholar
- Sadler, G., Chappas, W., Pierce, D.E.: Evaluation of e-beam, gamma- and X-ray treatment on the chemistry and safety of polymers used with pre-packaged irradiated foods: a review. Food Addit. Contam. 18(6), 475–501 (2001)Google Scholar
- Pop, E., Varshney, V., Roy, A.K.: Thermal properties of graphene: fundamentals and applications. MRS Bull. 37(12), 1273–1281 (2012)View ArticleGoogle Scholar
- Novoselov, K.S., et al.: Electric field effect in atomically thin carbon films. Science 306(5296), 666–669 (2004)View ArticleGoogle Scholar
- Shirafuji, J., Sugino, T.: Electrical properties of diamond surfaces. Diam. Relat. Mater. 5(6–8), 706–713 (1996)View ArticleGoogle Scholar
- Molitor, F., et al.: Energy and transport gaps in etched graphene nanoribbons. Semicond. Sci. Technol. 25(3), 034002 (2010)View ArticleGoogle Scholar
- Stampfer, C., et al.: Energy gaps in etched graphene nanoribbons. Phys. Rev. Lett. 102(5), 056403 (2009)View ArticleGoogle Scholar
- Shemella, P., et al.: Energy gaps in zero-dimensional graphene nanoribbons. Appl. Phys. Lett. 91(4), 042101 (2007)View ArticleGoogle Scholar
- Son, Y.W., Cohen, M.L., Louie, S.G.: Energy gaps in graphene nanoribbons. Phys. Rev. Lett. 97(21), 216803 (2006)View ArticleGoogle Scholar
- Hassanien, A., et al.: Geometrical structure and electronic properties of atomically resolved multiwall carbon nanotubes. Appl. Phys. Lett. 75(18), 2755–2757 (1999)View ArticleGoogle Scholar
- Wildoer, J.W.G., et al.: Electronic structure of atomically resolved carbon nanotubes. Nature 391(6662), 59–62 (1998)View ArticleGoogle Scholar
- Wang, Y., et al.: Resonance Raman spectroscopy of G-line and folded phonons in twisted bilayer graphene with large rotation angles. Appl. Phys. Lett. 103(12), 123101 (2013)View ArticleGoogle Scholar
- Wang, Y., et al.: Four-fold Raman enhancement of 2D band in twisted bilayer graphene: evidence for a doubly degenerate Dirac band and quantum interference. Nanotechnology 25(33), 335201 (2014)View ArticleGoogle Scholar
- Wang, J.-T., et al.: A new carbon allotrope with six-fold helical chains in all-sp2 bonding networks. Sci Rep 4, 4339 (2014)Google Scholar
- Calderon, H.A., et al.: Morphed graphene nanostructures: experimental evidence for existence. Carbon 102, 288–296 (2016)View ArticleGoogle Scholar
- Fals, A.E., Hadjiev, V.G., Robles, F.C.: Hernández, Multi-functional fullerene soot/alumina composites with improved toughness and electrical conductivity. Mater. Sci. Eng., A 558, 13–20 (2012)View ArticleGoogle Scholar
- Estrada-Guel, I., et al.: A green method for graphite exfoliation using high-energy ball milling. Microsc. Microanal. 21(S3), 615–616 (2015)Google Scholar
- Estrada-Guel, I., Robles-Hernandez, F., Martínez-Sánchez, R.: A green method for graphite exfoliation Using a mechanochemical route. Materials characterization, pp. 179–188. Springer International Publishing, New York City (2015)Google Scholar
- Estrada-Guel, I., et al.: A Green Method for Graphite Exfoliation, Effect of Milling Intensity. Micros Microanal 20(S3), 1780–1781 (2014)View ArticleGoogle Scholar
- Kisielowski, C., et al.: Real-time sub-Angstrom imaging of reversible and irreversible conformations in rhodium catalysts and graphene. Phys Rev B 88(2), 024305 (2013)View ArticleGoogle Scholar
- Kisielowski, C., et al.: Instrumental requirements for the detection of electron beam-induced object excitations at the single atom level in high-resolution transmission electron microscopy. Micron 68, 186–193 (2015)View ArticleGoogle Scholar
- Calderon, H.A., et al.: Maintaining the genuine structure of 2D materials and catalytic nanoparticles at atomic resolution. Micron 68, 164–175 (2015)View ArticleGoogle Scholar
- Gilman, P.S., Benjamin, J.S.: Mechanical alloying. Ann Rev Mater Sci 13, 279–300 (1983)View ArticleGoogle Scholar
- Robles Hernandez, F.C., Okonkwo, A., Benavides D.H.A.C.: Synthesis of effective carbon nanoreinforcements for structural applications. Houston U.O. (ed), p. 38. USA (2014)Google Scholar
- Cullity, B.D.: Elements of x-ray diffraction 2nd edn. In: Metallurgy and materials, p 555. Addison-Wesley Pub. Co. xii, Boston, (1978)Google Scholar
- Lavernia, E.J., Zhang, Z., Zhou, F.: On the analysis of grain size in bulk nanocrystalline materials via X-ray diffraction. Metall Mater Trans a-Phys Metall Mater Sci 34A(6), 1349–1355 (2003)Google Scholar
- Fals, A.E., Quintero, J., Hernández, F.C.R.: Manufacturing of hybrid composites and novel methods to synthesize carbon nanoparticles. MRS Online Proceed Librar 1276, 3 (2010)View ArticleGoogle Scholar
- Robles-Hernández, F., Calderón H.: Nanostructured Al-Al4C3 composites using C_Graphite or C_Fullerene as initial reinforcements. In: ICCE-16 Conference. Kungming (2008)Google Scholar
- Fals, A.E., Hadjiev, V.G., Hernandez, F.C.R.: Multi-functional fullerene soot/alumina composites with improved toughness and electrical conductivity. Mater Sci Eng Struct Mater Prop Microstruct Process 558, 13–20 (2012)View ArticleGoogle Scholar
- Robles Hernández, F.C., Calderón, H.A.: Synthesis of fullerene by spark plasma sintering and thermomechanical transformation of fullerene into diamond on Fe-C composites. In: MRS conference, MRS, Cancun (2010)Google Scholar
- Fals, A.E., Hadjiev, V.G., Robles, F.C.: Hernández, Porous media reinforced with carbon soots. Mater. Chem. Phys. 140(2–3), 651–658 (2013)View ArticleGoogle Scholar
- Santana, I.I., et al.: Fullerene-metal composites: phase transformations during milling and sintering. Solid State Phenom. 172–174, 727–732 (2011)View ArticleGoogle Scholar
- Ownby, P.D., Yang, X., Liu, J.: Calculated X-Ray-diffraction data for diamond polytypes. J. Am. Ceram. Soc. 75(7), 1876–1883 (1992)View ArticleGoogle Scholar
- Clark, S.J., et al.: First principles methods using CASTEP. Z. Kristallogr. 220, 567–570 (2005)Google Scholar
- Perdew, J.P., Burke, K., Ernzerhof, M.: Generalized gradient approximation made simple. Phys. Rev. Lett. 77(18), 3865–3868 (1996)View ArticleGoogle Scholar
- Monkhorst, H.J., Pack, J.D.: Special points for Brillouin-zone integrations. Phys Rev B 13(12), 5188–5192 (1976)View ArticleGoogle Scholar